LMucko/crystallography-open-database huggingface dataset:
Crystal structure and crystal chemistry of lithium-bearing muscovite-2M1 Sample: 2a
Brigatti, M. F.; Kile, D. E.; Poppi, M.; The Canadian Mineralogist 39 (2001) 1171–1180; doi:10.2113/gscanmin.39.4.1171

data_9004641
_publ_section_title
;
 Crystal structure and crystal chemistry of lithium-bearing muscovite-2M1
 Sample: 2a
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1171
_journal_page_last               1180
_journal_paper_doi               10.2113/gscanmin.39.4.1171
_journal_volume                  39
_journal_year                    2001
_chemical_formula_sum
'Al2.672 F0.28 Fe0.13 H1.72 K0.84 Li0.14 Mg0.01 Na0.14 O11.72 Rb0.02 Si3.128'
_chemical_name_mineral           Muscovite-2M1
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 95.71
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.197
_cell_length_b                   9.019
_cell_length_c                   20.068
_cell_volume                     935.955
_database_code_amcsd             0005734
_exptl_crystal_density_diffrn    2.844
_cod_original_formula_sum
'O11.72 (F.28 Na.14) Rb.02 K.84 Si3.128 Al2.672 Fe.13 Li.14 Mg.01 H1.72'
_cod_database_code               9004641
Crystal structure and crystal chemistry of lithium-bearing muscovite-2M1 O4 B33 is missing a zero Sample: 2b
Brigatti, M. F.; Kile, D. E.; Poppi, M.; The Canadian Mineralogist 39 (2001) 1171–1180; doi:10.2113/gscanmin.39.4.1171

data_9004642
_publ_section_title
;
 Crystal structure and crystal chemistry of lithium-bearing muscovite-2M1
 O4 B33 is missing a zero
 Sample: 2b
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1171
_journal_page_last               1180
_journal_paper_doi               10.2113/gscanmin.39.4.1171
_journal_volume                  39
_journal_year                    2001
_chemical_formula_sum
'Al2.568 F0.28 Fe0.13 H1.72 K0.84 Li0.13 Mg0.01 Na0.14 O11.72 Rb0.02 Si3.192'
_chemical_name_mineral           Muscovite-2M1
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 95.60
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.190
_cell_length_b                   9.022
_cell_length_c                   20.057
_cell_volume                     934.670
_database_code_amcsd             0005735
_exptl_crystal_density_diffrn    2.840
_cod_original_formula_sum
'O11.72 (F.28 Na.14) Rb.02 K.84 Si3.192 Al2.568 Fe.13 Li.13 Mg.01 H1.72'
_cod_database_code               9004642
Crystal structure and crystal chemistry of lithium-bearing muscovite-2M1 Sample: 147
Brigatti, M. F.; Kile, D. E.; Poppi, M.; The Canadian Mineralogist 39 (2001) 1171–1180; doi:10.2113/gscanmin.39.4.1171

data_9004643
_publ_section_title
;
 Crystal structure and crystal chemistry of lithium-bearing muscovite-2M1
 Sample: 147
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1171
_journal_page_last               1180
_journal_paper_doi               10.2113/gscanmin.39.4.1171
_journal_volume                  39
_journal_year                    2001
_chemical_formula_sum
'Al2.24 F0.42 Fe0.47 H1.58 K0.96 Li0.27 Na0.01 O11.58 Rb0.03 Si3.24'
_chemical_name_mineral           Muscovite-2M1
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 95.70
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.209
_cell_length_b                   9.038
_cell_length_c                   19.997
_cell_volume                     936.783
_database_code_amcsd             0005736
_exptl_crystal_density_diffrn    2.941
_cod_original_formula_sum
'O11.58 (F.42 Na.01) Rb.03 K.96 Si3.24 Al2.24 Fe.47 Li.27 H1.58'
_cod_database_code               9004643
Crystal structure and crystal chemistry of lithium-bearing muscovite-2M1 Sample: 129
Brigatti, M. F.; Kile, D. E.; Poppi, M.; The Canadian Mineralogist 39 (2001) 1171–1180; doi:10.2113/gscanmin.39.4.1171

data_9004644
_publ_section_title
;
 Crystal structure and crystal chemistry of lithium-bearing muscovite-2M1
 Sample: 129
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1171
_journal_page_last               1180
_journal_paper_doi               10.2113/gscanmin.39.4.1171
_journal_volume                  39
_journal_year                    2001
_chemical_formula_sum
'Al2.16 F0.58 Fe0.42 H1.42 K0.97 Li0.38 Mg0.01 Na0.02 O11.42 Rb0.01 Si3.28'
_chemical_name_mineral           Muscovite-2M1
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 95.63
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.224
_cell_length_b                   9.081
_cell_length_c                   19.952
_cell_volume                     941.940
_database_code_amcsd             0005737
_exptl_crystal_density_diffrn    2.899
_cod_original_formula_sum
'O11.42 (F.58 Na.02) Rb.01 K.97 Si3.28 Al2.16 Fe.42 Li.38 Mg.01 H1.42'
_cod_database_code               9004644
The crystal chemistry of the [M3_11-14] trimeric structures: From hyperagpaitic complexes to saline lakes
Sokolova, E. V.; Hawthorne, F. C.; The Canadian Mineralogist 39 (2001) 1275–1294; doi:10.2113/gscanmin.39.5.1275

data_9004645
_publ_section_title
;
 The crystal chemistry of the [M3_11-14] trimeric structures:
 From hyperagpaitic complexes to saline lakes
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1275
_journal_page_last               1294
_journal_paper_doi               10.2113/gscanmin.39.5.1275
_journal_volume                  39
_journal_year                    2001
_chemical_formula_sum            'Ca1.96 F2 Na4.04 O8 P2'
_chemical_name_mineral           Nacaphite
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                90.002
_cell_angle_beta                 89.998
_cell_angle_gamma                89.965
_cell_length_a                   5.3232
_cell_length_b                   12.2103
_cell_length_c                   7.0961
_cell_formula_units_Z            2
_cell_volume                     461.231
_database_code_amcsd             0005738
_exptl_crystal_density_diffrn    2.876
_cod_original_formula_sum        'Ca1.96 Na4.04 P2 F2 O8'
_cod_database_code               9004645
The crystal chemistry of the [M3_11-14] trimeric structures: From hyperagpaitic complexes to saline lakes
Sokolova, E. V.; Hawthorne, F. C.; The Canadian Mineralogist 39 (2001) 1275–1294; doi:10.2113/gscanmin.39.5.1275

data_9004646
_publ_section_title
;
 The crystal chemistry of the [M3_11-14] trimeric structures:
 From hyperagpaitic complexes to saline lakes
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1275
_journal_page_last               1294
_journal_paper_doi               10.2113/gscanmin.39.5.1275
_journal_volume                  39
_journal_year                    2001
_chemical_formula_sum
'Ca1.44 F2 Fe0.1 Mg0.5 Mn0.85 Na13.59 Nb0.44 O34 P4 Si4 Sr0.06 Ti2.55 Zr0.47'
_chemical_name_mineral           Quadruphite
_space_group_IT_number           1
_symmetry_space_group_name_Hall  'P 1'
_symmetry_space_group_name_H-M   'P 1'
_cell_angle_alpha                86.89
_cell_angle_beta                 94.42
_cell_angle_gamma                89.94
_cell_length_a                   5.4206
_cell_length_b                   7.0846
_cell_length_c                   20.3641
_cell_formula_units_Z            1
_cell_volume                     778.553
_database_code_amcsd             0005739
_exptl_crystal_density_diffrn    3.122
_cod_original_formula_sum
'Ti2.55 Nb.44 Zr.47 Mn.85 Fe.1 Na13.59 Mg.5 Ca1.44 Sr.06 P4 Si4 F2 O34'
_cod_database_code               9004646
Natrolemoynite, a new hydrated sodiium zirconosilicate from Mont Saint-Hilaire, Quebec: Description and structure determination Locality: Mont Saint-Hilaire, Quebec, Canada
McDonald, A. M.; Chao, G. Y.; The Canadian Mineralogist 39 (2001) 1295–1306; doi:10.2113/gscanmin.39.5.1295

data_9004647
_publ_section_title
;Natrolemoynite, a new hydrated sodiium zirconosilicate from Mont
 Saint-Hilaire, Quebec: Description and structure determination Locality: Mont
 Saint-Hilaire, Quebec, Canada
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1295
_journal_page_last               1306
_journal_paper_doi               10.2113/gscanmin.39.5.1295
_journal_volume                  39
_journal_year                    2001
_chemical_compound_source        'Mont Saint-Hilaire, Quebec, Canada'
_chemical_formula_sum
'Ca0.01 H2.42 K0.05 Na1.44 Nb0.04 O17.56 Si5 Ti0.02 Zr0.94'
_chemical_name_mineral           Natrolemoynite
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 105.462
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   10.5150
_cell_length_b                   16.2534
_cell_length_c                   9.1029
_cell_volume                     1499.421
_database_code_amcsd             0005740
_exptl_crystal_density_diffrn    2.435
_cod_original_formula_sum
'Na1.44 K.05 Ca.01 (Zr.94 Nb.04 Ti.02) Si5 O17.56 H2.42'
_cod_database_code               9004647
The crystal structure of delindeite, Ba2{(Na,K,_)3(Ti,Fe)[Ti2(O,OH)4Si4O14](H2O,OH)2}, a member of the mero-plesiotype bafertisite series
Ferraris, G.; Ivaldi, G.; Pushcharovsky, D. Y.; Zubkova, N. V.; Pekov, I. V.; The Canadian Mineralogist 39 (2001) 1307–1316; doi:10.2113/gscanmin.39.5.1307

data_9004648
_publ_section_title
;The crystal structure of delindeite,
 Ba2{(Na,K,_)3(Ti,Fe)[Ti2(O,OH)4Si4O14](H2O,OH)2}, a member of the
 mero-plesiotype bafertisite series
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1307
_journal_page_last               1316
_journal_paper_doi               10.2113/gscanmin.39.5.1307
_journal_volume                  39
_journal_year                    2001
_chemical_formula_sum            'Ba2 H8 Na1.6 O19.92 Si4 Ti3'
_chemical_name_mineral           Delindeite
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-A 2y'
_symmetry_space_group_name_H-M   'A 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 93.80
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.327
_cell_length_b                   6.856
_cell_length_c                   21.51
_cell_volume                     783.859
_database_code_amcsd             0005741
_exptl_crystal_density_diffrn    3.789
_cod_original_formula_sum        'Ba2 Ti3 Si4 Na1.6 O19.92 H8'
_cod_database_code               9004648
The crystal structure of baricite, (Mg1.70Fe1.30)(PO4)2.8H2O
Yakubovich, O. V.; Massa, W.; Liferovich, R. P.; McCammon, C. A.; The Canadian Mineralogist 39 (2001) 1317–1324; doi:10.2113/gscanmin.39.5.1317

data_9004649
_publ_section_title
;
 The crystal structure of baricite, (Mg1.70Fe1.30)(PO4)2.8H2O
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1317
_journal_page_last               1324
_journal_paper_doi               10.2113/gscanmin.39.5.1317
_journal_volume                  39
_journal_year                    2001
_chemical_formula_sum            'Fe1.3 H16 Mg1.7 O16 P2'
_chemical_name_mineral           Baricite
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 104.96
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   10.085
_cell_length_b                   13.390
_cell_length_c                   4.6713
_cell_volume                     609.423
_database_code_amcsd             0005742
_exptl_crystal_density_diffrn    2.441
_cod_original_formula_sum        '(Fe1.3 Mg1.7) P2 O16 H16'
_cod_database_code               9004649
Orthominasragrite, VO(SO4)(H2O)5, a new mineral species from Temple Mountain, Emery county, Utah, U.S.A.
Hawthorne, F. C.; Schindler, M.; Grice, J. D.; Haynes, P.; The Canadian Mineralogist 39 (2001) 1325–1331; doi:10.2113/gscanmin.39.5.1325

data_9004650
_publ_section_title
;
 Orthominasragrite, VO(SO4)(H2O)5, a new mineral species from Temple
 Mountain, Emery county, Utah, U.S.A.
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1325
_journal_page_last               1331
_journal_paper_doi               10.2113/gscanmin.39.5.1325
_journal_volume                  39
_journal_year                    2001
_chemical_compound_source        'Temple Mountain, Emery county, Utah, USA'
_chemical_formula_sum            'H10 O10 S V'
_chemical_name_mineral           Orthominasragrite
_space_group_IT_number           31
_symmetry_space_group_name_Hall  'P 2ac -2'
_symmetry_space_group_name_H-M   'P m n 21'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.242
_cell_length_b                   9.319
_cell_length_c                   6.192
_cell_volume                     417.887
_database_code_amcsd             0005743
_exptl_crystal_density_diffrn    2.011
_cod_depositor_comments
;

2017-09-06
Z value inserted to be consistent with given formula
Water oxygens renamed so they are recognized as oxygens
                 miguel
;
_cod_original_formula_sum        'V S O10 H10'
_cod_database_code               9004650
Crystal chemistry of trioctahedral micas - 1M from the Alto Paranaiba Igneous Province, Southeastern Brazil Sample: Tpp16-6a
Brigatti, M. F.; Medici, L.; Poppi, L.; Vaccaro, C.; The Canadian Mineralogist 39 (2001) 1333–1345; doi:10.2113/gscanmin.39.5.1333

data_9004651
_publ_section_title
;
 Crystal chemistry of trioctahedral micas - 1M from the Alto Paranaiba
 Igneous Province, Southeastern Brazil
 Sample: Tpp16-6a
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1333
_journal_page_last               1345
_journal_paper_doi               10.2113/gscanmin.39.5.1333
_journal_volume                  39
_journal_year                    2001
_chemical_compound_source
'Alto Paranaiba Igneous Province, Southeastern Brazil'
_chemical_formula_sum
'Al1.04 F0.12 Fe0.37 H1.88 K0.98 Mg2.73 Na0.01 O11.88 Si2.8 Ti0.06'
_chemical_name_mineral           Phlogopite
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 99.89
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.330
_cell_length_b                   9.239
_cell_length_c                   10.305
_cell_volume                     499.917
_database_code_amcsd             0005744
_exptl_crystal_density_diffrn    2.853
_cod_original_formula_sum
'O11.88 (F.12 Si2.8) Al1.04 Fe.37 Mg2.73 Ti.06 Na.01 K.98 H1.88'
_cod_database_code               9004651
Crystal chemistry of trioctahedral micas - 1M from the Alto Paranaiba Igneous Province, Southeastern Brazil Sample: Tax27-1, ferroan
Brigatti, M. F.; Medici, L.; Poppi, L.; Vaccaro, C.; The Canadian Mineralogist 39 (2001) 1333–1345; doi:10.2113/gscanmin.39.5.1333

data_9004652
_publ_section_title
;
 Crystal chemistry of trioctahedral micas - 1M from the Alto Paranaiba
 Igneous Province, Southeastern Brazil
 Sample: Tax27-1, ferroan
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1333
_journal_page_last               1345
_journal_paper_doi               10.2113/gscanmin.39.5.1333
_journal_volume                  39
_journal_year                    2001
_chemical_compound_source
'Alto Paranaiba Igneous Province, Southeastern Brazil'
_chemical_formula_sum
'Al0.8 F0.04 Fe0.72 H1.96 K0.95 Mg2.43 Na0.03 O11.96 Si2.96 Ti0.09'
_chemical_name_mineral           Phlogopite
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 99.99
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.351
_cell_length_b                   9.267
_cell_length_c                   10.311
_cell_volume                     503.547
_database_code_amcsd             0005745
_exptl_crystal_density_diffrn    2.903
_cod_original_formula_sum
'O11.96 (F.04 Si2.96) Al.8 Fe.72 Mg2.43 Ti.09 Na.03 K.95 H1.96'
_cod_database_code               9004652
Crystal chemistry of trioctahedral micas - 1M from the Alto Paranaiba Igneous Province, Southeastern Brazil Sample: Taa11-1A, ferroan T-O3 given as 1.663, but I compute 1.647
Brigatti, M. F.; Medici, L.; Poppi, L.; Vaccaro, C.; The Canadian Mineralogist 39 (2001) 1333–1345; doi:10.2113/gscanmin.39.5.1333

data_9004653
_publ_section_title
;
 Crystal chemistry of trioctahedral micas - 1M from the Alto Paranaiba
 Igneous Province, Southeastern Brazil
 Sample: Taa11-1A, ferroan
 T-O3 given as 1.663, but I compute 1.647
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1333
_journal_page_last               1345
_journal_paper_doi               10.2113/gscanmin.39.5.1333
_journal_volume                  39
_journal_year                    2001
_chemical_compound_source
'Alto Paranaiba Igneous Province, Southeastern Brazil'
_chemical_formula_sum
'Al1.12 F0.04 Fe0.7 H1.84 K0.98 Mg2.25 Na0.02 O11.96 Si2.84 Ti0.09'
_chemical_name_mineral           Phlogopite
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 99.97
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.329
_cell_length_b                   9.244
_cell_length_c                   10.271
_cell_volume                     498.322
_database_code_amcsd             0005746
_exptl_crystal_density_diffrn    2.938
_cod_original_formula_sum
'O11.96 F.04 Si2.84 Al1.12 Fe.7 Mg2.25 Ti.09 (Na.02 K.98) H1.84'
_cod_database_code               9004653
Crystal chemistry of trioctahedral micas - 1M from the Alto Paranaiba Igneous Province, Southeastern Brazil Sample: Tai17-1, ferroan
Brigatti, M. F.; Medici, L.; Poppi, L.; Vaccaro, C.; The Canadian Mineralogist 39 (2001) 1333–1345; doi:10.2113/gscanmin.39.5.1333

data_9004654
_publ_section_title
;
 Crystal chemistry of trioctahedral micas - 1M from the Alto Paranaiba
 Igneous Province, Southeastern Brazil
 Sample: Tai17-1, ferroan
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1333
_journal_page_last               1345
_journal_paper_doi               10.2113/gscanmin.39.5.1333
_journal_volume                  39
_journal_year                    2001
_chemical_compound_source
'Alto Paranaiba Igneous Province, Southeastern Brazil'
_chemical_formula_sum
'Al1.12 Ba0.01 Fe0.62 H1.88 K0.98 Mg2.37 Na0.02 O12 Si2.8 Ti0.09'
_chemical_name_mineral           Phlogopite
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 99.94
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.3355
_cell_length_b                   9.2457
_cell_length_c                   10.294
_cell_volume                     500.185
_database_code_amcsd             0005747
_exptl_crystal_density_diffrn    2.918
_cod_original_formula_sum
'O12 Si2.8 Al1.12 Fe.62 Mg2.37 Ti.09 Na.02 K.98 Ba.01 H1.88'
_cod_database_code               9004654
Crystal chemistry of trioctahedral micas - 1M from the Alto Paranaiba Igneous Province, Southeastern Brazil Sample: Ta9, ferroan
Brigatti, M. F.; Medici, L.; Poppi, L.; Vaccaro, C.; The Canadian Mineralogist 39 (2001) 1333–1345; doi:10.2113/gscanmin.39.5.1333

data_9004655
_publ_section_title
;
 Crystal chemistry of trioctahedral micas - 1M from the Alto Paranaiba
 Igneous Province, Southeastern Brazil
 Sample: Ta9, ferroan
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1333
_journal_page_last               1345
_journal_paper_doi               10.2113/gscanmin.39.5.1333
_journal_volume                  39
_journal_year                    2001
_chemical_compound_source
'Alto Paranaiba Igneous Province, Southeastern Brazil'
_chemical_formula_sum
'Al0.92 Ba0.02 F0.02 Fe1.22 H1.82 K0.98 Mg1.74 Mn0.03 O11.98 Si3 Ti0.09'
_chemical_name_mineral           Phlogopite
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 100.01
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.344
_cell_length_b                   9.259
_cell_length_c                   10.280
_cell_volume                     500.912
_database_code_amcsd             0005748
_exptl_crystal_density_diffrn    3.053
_cod_original_formula_sum
'O11.98 F.02 Si3 Al.92 Fe1.22 Mg1.74 Ti.09 Mn.03 (K.98 Ba.02) H1.82'
_cod_database_code               9004655
Crystal chemistry of trioctahedral micas - 1M from the Alto Paranaiba Igneous Province, Southeastern Brazil Sample: Li12a, ferroan
Brigatti, M. F.; Medici, L.; Poppi, L.; Vaccaro, C.; The Canadian Mineralogist 39 (2001) 1333–1345; doi:10.2113/gscanmin.39.5.1333

data_9004656
_publ_section_title
;
 Crystal chemistry of trioctahedral micas - 1M from the Alto Paranaiba
 Igneous Province, Southeastern Brazil
 Sample: Li12a, ferroan
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1333
_journal_page_last               1345
_journal_paper_doi               10.2113/gscanmin.39.5.1333
_journal_volume                  39
_journal_year                    2001
_chemical_compound_source
'Alto Paranaiba Igneous Province, Southeastern Brazil'
_chemical_formula_sum
'Al0.92 F0.18 Fe0.53 H1.72 K0.95 Mg2.52 Na0.04 O11.82 Si3 Ti0.03'
_chemical_name_mineral           Phlogopite
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 99.96
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.331
_cell_length_b                   9.227
_cell_length_c                   10.275
_cell_volume                     497.801
_database_code_amcsd             0005749
_exptl_crystal_density_diffrn    2.893
_cod_original_formula_sum
'O11.82 F.18 Si3 Al.92 Fe.53 Mg2.52 Ti.03 Na.04 K.95 H1.72'
_cod_database_code               9004656